### GEORGIAN ACADEMY OF NATURAL SCIENCES

### TBILISI INTERNATIONAL CENTRE OF MATHEMATICS AND INFORMATICS

**L E C T U R E** **N O T E S** **of**

**of**

**T I C M I**

### Tbilisi

### Volume 16, 2015

** AND SIMULATIONS**

**PHENOMENOLOGY, THEORY, APPLICATIONS,** **STRUCTURAL CHANGES IN MICRO-MATERIALS:**

**W.H. Mü ** **ller, E.N. Vilchevskaya, & A.B. Freidin**

M. Sharikadze

**Abstracted/Indexed in:** Mathematical Reviews, Zentralblatt Math
Iv. Javakhishvili Tbilisi State University

David Natroshvili, Tbilisi, Georgian Technical University

Alexander Meskhi, Tbilisi, A. Razmadze Mathematical Institute, Tbilisi State University

**Editor:**G. Jaiani

I. Vekua Institute of Applied Mathematics Tbilisi State University

2, University St., Tbilisi 0186, Georgia Tel.: (+995 32) 218 90 98

e.mail: george.jaiani@viam.sci.tsu.ge

Vaxtang Kvaratskhelia, Tbilisi, N. Muskhelishvili Institute of Computational Mathematics Olga Gil-Medrano, Valencia, Universidad de Valencia

**Cover Designer:**N. Ebralidze
**English Editor:** Ts. Gabeskiria

**Managing Editor:**N. Chinchaladze

**Technical editorial board:**M. Tevdoradze

**Websites: http://www.viam.science.tsu.ge/others/ticmi/lnt/lecturen.htm**
http://www.emis.de/journals/TICMI/lnt/lecturen.htm

Courses and Workshops organized by TICMI (Tbilisi International Center of Mathematics and Informatics). The advanced courses cover the entire field of mathematics (especially of its applications to mechanics and natural sciences) and from informatics which are of interest to postgraduate and PhD students and young scientists.

**International Scientific Committee of TICMI:**

Alice Fialowski, Budapest, Institute of Mathematics, Pazmany Peter setany 1/C Pedro Freitas, Lisbon, University of Lisbon

George Jaiani (Chairman), Tbilisi, I.Vekua Institute of Applied Mathematics,

**© TBILISI UNIVERSITY PRESS, 2015**

**1** **Microstructural changes in modern electronic materials** **7**

**2** **Silicon oxidation** **8**

2.1 The technical perspective . . . 8

2.2 Quantifying the volume expansion . . . 10

2.3 Modeling the residual strains and stresses . . . 12

2.4 Intuitive explanations and empirical quantification of the imped- iment encountered during silicon oxidation . . . 17

2.5 Driving forces at the reaction front . . . 18

2.6 Mathematical treatment of silicon oxidation – The full picture 22 2.6.1 Relevant kinematic quantities . . . 22

2.6.2 Mass densities . . . 23

2.6.3 Stress tensors . . . 25

2.6.4 Chemical affinities and their jumps – The general case . 26 2.6.5 Normal speed of the interface . . . 27

2.6.6 Specialization to Hookean solids and ideal gases . . . 28

2.6.7 Equilibrium and diffusion . . . 29

2.7 Case study – A two-dimensional planar reaction front . . . 31

2.7.1 Problem description . . . 31

2.7.2 Solution of the elasticity problem for prescribed displace- ments . . . 31

2.7.3 Solution of the elasticity problem for prescribed stresses 34 2.7.4 Solution of the diffusion problem . . . 37

2.7.5 Materials data . . . 38

2.7.6 Results for prescribed displacements . . . 41

2.7.7 Results for prescribed stresses . . . 42

**3** **Spinodal decomposition** **44**
3.1 Phenomenology . . . 44

3.2 Mathematical treatment of spinodal decomposition . . . 48

3.2.1 Setting the stage . . . 48

3.2.2 The mechanical part of the model - Basic relations . . . 49 3.2.3 The mechanical part of the model - Numerical approach 50

3.2.4 The thermodynamics part of the model - Basic relations 54 3.2.5 The thermodynamics part of the model - Numerical ap-

proach . . . 54

3.2.6 A few words regarding the material parameters . . . 55

3.3 Simulations . . . 57

3.3.1 Initial conditions . . . 57

3.3.2 Aging at high and low temperatures . . . 57

3.3.3 Simulation of temperature cycling . . . 58

3.3.4 Influence of surface tensions . . . 59

3.3.5 Influence of external stress and potential healing . . . . 59

**4** **Growth of intermetallic compounds** **60**
4.1 Phenomenology . . . 60

4.2 Reliability issues . . . 61

4.3 The modeling-state-of-the-art . . . 63

on the (sub-) microscale of materials used in today’s microelectronic technology and have an impact on the manufacturing process as well as the reliability of the whole electronic structure.

The first example concerns the oxidation process of silicon. The formation
of silicon oxide out of silicon is accompanied by mechanical deformation due to
a change of volume during the reaction. The developing stresses and strains
influence the diffusion kinetics of the process: They can even bring it to
a standstill. Material scientists tend to model the mechanical part of the
phenomenon by adding an artificial stress dependence to the diffusion and to
the reaction constants. In this paper we will pursue a different approach based
on a sharp interface model. Starting from first principles an expression for the
velocity of the oxidation front will be derived. The front velocity is related to
the local Eshelby tensor and contains *a priori* chemical as well as mechanical
driving forces.

The second example deals with the aging of eutectic tin-lead solder. This
is a two-phase material consisting of regions rich in tin and regions rich in
lead because tin and lead mix only very slightly. Initially these regions are
finely dispersed giving rise to a filigreed micro-structure, *i.e.*, an electrically
and mechanically highly reliable solder joint has been generated. However,
due to temperature and the presence of local mechanical stresses a solid →
solid diffusion process sets in and the regions start coarsening. The micro-
structure deteriorates and the solder joints eventually becomes electrically
and mechanically unreliable. A phase-field model will be used to describe the
process of spinodal decomposition.

The third and final example addresses the formation and the ripening of
intermetallic phases in microelectronic solders or at the interface between the
solder and the connecting pad. The formation of such phases is accompanied
by a change in volume just like during the formation of silicon dioxide. In other
words, this is another example of stress-assisted growth kinetics. However,
other than silicon dioxide they show a highly ordered crystalline structure, *i.e.*,
they are anisotropic which, in particular, influences their growth behavior. The
paper will end with a discussion of potential models that could be used for a
quantitative description.

**2000 Mathematical Subject Classification:** 74B10, 74N20, 74N25, 74S25

**Key words and phrases:** micro-materials, evolving microstructure, stress-
driven diffusion

**Wolfgang H. Müller**^{∗}

Technische Universität Berlin, Institut für Mechanik, LKM, Einsteinufer 5, 13591 Berlin, Germany

**Elena N. Vilchevskaya**^{a,b} **and Alexander B. Freidin**^{a,c}

aInstitute for Problems in Mechanical Engineering of Russian Academy of Sciences, Bolshoy Pr., 61, V.O., St. Petersburg 199178, Russia

bSt. Petersburg State Polytechnical University, Polytechnicheskaya Str., 29, St. Petersburg 195251, Russia

Received 15.09.2015; Revised 20.10.2015; Accepted 28.10.2015

∗ Corresponding author. Email: wolfgang.h.mueller@tu-berlin.de

cSt. Petersburg State University, Universitetsky Pr., 28, Peterhof, St. Petersburg 198504, Russia

The development of modern electronic and mechatronic products is dictated by the continuous quest toward further and further miniaturization. Consequently, the microstructure of the production materials is of paramount importance.

Moreover, once a certain beneficial microstructure has been realized it is by no means guaranteed that it will continue to exist the way it was initially created. We face a dynamic situation during which the structure may change and, consequently, reliability issues due to aging of the materials will arise.

All of this is bad news for the manufacturers of products. However, it results in challenging tasks for material scientists, physicists, and mathematicians, all of whose skills are required for a better understanding and for the mathematical description of the underlying chemistry and physics.

In what follows we will focus on three phenomena which, as we shall see, are
related in terms of microstructural change and the corresponding mathematical
modeling. In each case we will first present the experimental evidence and
try to explain the findings verbally. The latter will guide us during the setup
of an appropriate mathematical model. We will then spend a considerable
amount of time to make these models as quantitative as possible. In other
words, it will be our goal to find data for the involved material parameters
not by matching the experiments to the model but from independent sources
unrelated to the phenomenon in question. Note that there is a fundamental
difference between our approach and the commonly adopted materials science
point-of-view. The latter is frequently *ad hoc*, in the sense that parameters
are “adjusted” so that the model eventually leads to the required outcome.

Of course, materials scientists attempt to motivate their adjustment of model parameters. However, their efforts are often heuristic, based exclusively on words and not on first principles in terms of physics combined with adequate mathematical techniques. Moreover, once an adjustment has been brought to perfect coincidence with the experimental findings in one situation it is by no means guaranteed that the same set of parameters can be used for another geometry. This, however, is a measure of the quality of a model in the sense of a true capture of the behavior of nature.

**2.1** **The technical perspective**

Following the nomenclature established in [28] we consider a binary reaction of the type:

*𝑛*−*𝐵*−+*𝑛*∗*𝐵*∗⇌*𝑛*+*𝐵*+ (2.1.1)
and apply it to the so-called *dry* oxidation process of silicon, *i.e.*,

Si+O2⇌SiO2*.* (2.1.2)

The symbols *𝑛*− , *𝑛*∗, and *𝑛*+, which are known under the term *stoichiometric*
*coefficients*, characterize the number of atoms or molecules of the reactants and
of the products involved in the reaction. They are pure numbers without a
unit, but they do have a sign [40]: Reactants, *i.e.*, the *𝑛*’s on the left hand side
of the reaction balance, are counted negatively, whereas the products on the
right hand side have positive values. The *𝑛*’s should also not be confused with
the so-called *chemical amount* of a substance, which is also frequently used in
chemical thermodynamics in context with reaction equations. Following the
conventions of chemical engineers these “amounts” have a unit, namely 1 mol
or 1 kmol, depending on whether we count mass in g or in kg.

Figure 2.1: A schematic of dry silicon oxidation, see [69] for details.

In the case of dry oxidation of silicon we have*𝑛*−≡*𝑛*Si= −1,*𝑛*∗≡*𝑛*_{O2} = −1,
and*𝑛*+≡*𝑛*_{SiO2} = +1. Note that we do not write *𝑛*∗≡*𝑛*O= −2, because this is*not*
the elementary reaction taking place at the atomic scale: An oxygen molecule
diffuses from the outside to the silicon surface where it links with a silicon
atom and forms one silicon dioxide “molecule.” Then several such aggregates
form an amorphous layer of silicon dioxide or silica which grows continuously:

Fig. 2.1. Clearly the diffusion of the outside oxygen molecules to reach the
*current* silicon surface will take more time the thicker the amorphous layer
becomes. However, rumor has it that the oxygen molecules are not severely
impeded by the presence of the growing layer of silicon dioxide and that after
a very short time a stationary diffusion flow is established which, timewise, is
governed by a simple isotropic diffusion constant. We will get back to this issue

later, where we shall also discuss as to whether the diffusion constant might
be *anisotropic*, that it might be affected by mechanical stress and strain, and

“how fast” it is in comparison with relaxation processes within the amorphous layer.

Figure 2.2: Schematics of the LOCOS and STI processes, see [38] for details.

For completeness note that there is an alternative process for creating silica,
namely the so-called *wet* oxidation:

Si+2H2O⇌SiO2+H2*.* (2.1.3)
Clearly this does not fit into the reaction scheme of Eqn. (2.1.1), since two
products result. Moreover, two water molecules have to interact with one silicon
atom instead of just one oxygen molecule. We will not model wet oxidation in
this paper. However, it should be mentioned at this point that either way a
relatively high temperature is required for the chemical reactions to take place.

Therefore they are also referred to as*thermal oxidation processes*. We will get
back to the temperature issue later.

Wet and dry oxidation were initially used in the eighties for*electric isolation*
of adjacent structures in microelectronic devices. In order to see that these
processes are effective and truly reach this goal we only need to look at the
electrical conductivities of SiO2 and Si, which are 10^{−16}Ω^{−1}cm^{−1} compared to
1*.*56×10^{−3}Ω^{−1}cm^{−1} [83], [94].

Presumably the first process of this kind on an industrial scale was LOCOS
(LOCal Oxidation of Silicon, *cf.*, [95]). This acronym refers to a microfabri-
cation scheme where silicon dioxide is formed in selected areas on a silicon
wafer having the Si-SiO2 interface at a lower point than the rest of the silicon
surface (*cf.*, Fig. 2.2). LOCOS is typically performed at temperatures between
800 and 1200^{○}C. However, it turned out that if the isolation windows became
narrower than 0*.*7μm oxide growth became progressively inhibited and would
result in oxide layers as much as 80 percent thinner than comparable layers
grown in wide windows greater than 2μm. “This is the so-called ‘oxide thinning
effect‘. [. . . ] Thinner-than-desired field oxide layers may allow widely different
breakdown and isolation characteristics between neighboring devices, and hence
seriously degrade device performance.” [46] The requirement for further minia-
turization outdated LOCOS and was superseded by Shallow Trench Isolation

(a) Schematic of nanowire fabrication (b) Nanosize tip

Figure 2.3: Silicon nanostructures. For details of (a) see [74], for (b) see [75].

(STI). STI is used on CMOS (Complementary Metal-Oxide-Semiconductor) process technology nodes of 250 nanometers and smaller. The range of applied temperatures is similar to that of LOCOS. “This process basically involves shallow trenching of the surface areas which are to be oxidized so as to obtain, as closely as possible, a planar surface after oxide growth. A very difficulty experienced in such steeped structures is that the oxide thickness on the edges are in the corners of trench can be much less than on flat surface. This is quite similar to thinning problems encountered in LOCOS structures.” [46]

More recently silicon oxidation has been used to manufacture extremely small silicon structures on the nanoscale. Two examples are shown in Fig. 2.3:

The manufacturing steps of silicon wires ranging from 200 to 20 nm in diameter
[70] and a real nanosize silicon tip [75]. The oxidation process of such nanosilicon
structures is typically performed at 850^{○}C (*cf.*, [33]) or 950^{○}C (*cf.*, [71]), *i.e.*,
at temperatures similar to those used for LOCOS and STI. Interestingly the
nanosize silicon beams buckle without external loads being applied. We shall
see now that this behavior has the same cause as the insufficient oxide layer
thickness described in context with LOCOS and STI.

**2.2** **Quantifying the volume expansion**

In order to understand and interpret these facts we must first realize that
the reaction described by Eqn. (2.1.2) is accompanied by a change in volume
and, consequently, by generating eigenstrains and eigenstresses. The latter are
sometimes also referred to as residual stresses in the engineering literature. To
be specific, according to Kao in 1988 *et al.* [42], pg. 29, the unit cell of silicon
is 20 Å^{3}, whereas that of silicon dioxide is 45 Å^{3}. Note that in [42] it is not
explained where these numbers come from. If such a large increase in volume
is correct, the resulting eigenstrains will be enormous. Thus, before we engage

in a discussion which kind of strain measure should be used for quantification, the validity of the data provided in [42] should be carefully checked.

A difference of *𝑉** _{𝑘}*=25 Å

^{31}between the two unit cell volumes is mentioned by Sutardja and Oldham in 1989 [87], pg. 2415. The agreement with Kao

*et al.*

[42] is not surprising, since they use that paper as a reference. However, it is
argued by them that a more proper value for the difference should be 12*.*5 Å^{3}
which, supposedly, is related to the difference between the distances of an Si-O
(not SiO2) and a Si-Si bond. Then it is said in [87] that “... The actual value of
*𝑉** _{𝑘}* used is obtained through numerical experiments, and the theoretical value
of 12

*.*5 Å

^{3}is used as a test for the validity of the model.” We strongly oppose to such a notion: A model should never be fitted to experiments, because then it is not a valid representation of reality. We therefore turn to the most detailed data survey presented in Mohr

*et al.*[51], pg. 681 to find that the unit cell volume of Si is indeed 12

*.*0588349×10

^{−}

^{3 m}

^{3}⇑

^{kmol}, hence,

*𝑉*

_{Si}= 12.0588349×10

^{−6}m

^{3}⇑kmol

*𝑁*Avo ≈20 Å^{3}.
Finding a reliable value for the molecular volume of SiO2 is more tedious.

Valuable guides are, first, the Wikipedia article on silicon dioxide, [97] and,
second, the discussion on ResearchGate, [77]. From both we realize that the
silicon dioxide of our microelectronics application is not “quartz” but rather the
amorphous variant of silicon dioxide. Moreover, note that Si has a mass density
of 2329^{kg}⇑^{m}^{3} (at room temperature, [75]) and, as mentioned in the previous
references, quartz, or more precisely Si3O6, has a mass density of 2648^{kg}⇑^{m}^{3},
whereas the mass density of amorphous SiO2 is only about 2200^{kg}⇑^{m}^{3}. The mass
density of liquid SiO2 is even less, namely approximately 2020^{kg}⇑^{m}^{3}. The molar
masses of silicon and silicon dioxide are easily obtained from Mendeleev’s table
of elements, namely, *𝑀*Si =28*.*084^{kg}⇑^{kmol} and *𝑀*_{SiO2} =60*.*082_{kmol}^{kg} , respectively.

In this paper we will use *𝑁*Avo=6*.*02214129×10^{26 1}⇑^{kmol}for Avogadro’s number.^{2}
In combination with the mass densities and Avogadro’s number we now obtain
for the unit cell volumes:

*𝑉*Si= *𝑀*Si

*𝜌*Si*𝑁*Avo

≈20*.*0 Å^{3} *,* *𝑉*_{SiO2}= *𝑀*_{SiO2}
*𝜌*_{SiO2}*𝑁*Avo

≈45*.*3 Å^{3}*.* (2.2.1)
This, at last, gives us more confidence in the numbers for the volume changes
presented by Kao *et al.* [42]. If we omit Avogadro’s number in the last equation
we obtain the so-called molar volumes:

*𝑣*Si= *𝑀*Si

*𝜌*Si

≈0*.*012_{kmol}^{m}^{3} *,* *𝑣*_{SiO2} = *𝑀*_{SiO2}

*𝜌*_{SiO2} ≈0*.*027_{kmol}^{m}^{3} *.* (2.2.2)
This confirms the statement in Rao and Hughes [72] according to which the

“molar volume of silicon dioxide is 2.2 times that of silicon.” The numbers also

1The index *𝑘* refers to the surface reaction rate parameter *𝑘* from [87], for which the
difference in volume is used in an Arrhenius ansatz.

2Note that molar masses have an SI-unit, namely g⇑mol or kg⇑kmol, [96]. Moreover, for
the sake of clarity, we should use ^{particles}⇑kmolas units of the Avogadro number. However,

“particles” is no official SI-unit.

agree with the following data that was provided in Freidin *et al.* [28] without
reference: ^{𝜌}^{Si}⇑^{𝑀}^{Si}=82*.*9^{kmol}⇑^{m}^{3} and^{𝜌}^{SiO2}⇑* ^{𝑀}*SiO2 =36

*.*6

^{kmol}⇑

^{m}

^{3}. In combination with the molar masses this, in turn, leads to density values of

*𝜌*Si=2328

^{kg}⇑

^{m}

^{3}and

*𝜌*

_{SiO2}=2199

^{kg}⇑

^{m}

^{3}, respectively, which essentially agrees with the data in the wikis on silicon, [98] and [97]. By using Avogadro’s constant we can convert this data also into unit cell volumes,

*𝑉*Si=20

*.*0 Å

^{3}and

*𝑉*

_{SiO2}=45 Å

^{3}, respectively.

This clearly indicates that the data of Kao *et al.* [42] were initially used in
Freidin *et al.* [28] and then transformed accordingly. In other words, one went
in circles as far as the unit cell data for amorphous silicon dioxide is concerned.

In summary, we may say that, first, the molar masses of Si and SiO2

are reliable. Second, the unit cell of silicon has been accurately examined by
crystallographic methods using X-ray techniques by Mohr*et al.* [51]. Third, the
silica resulting from the oxidation process has been identified as the amorphous
form. Fourth, the mass density of amorphous silica has been determined
experimentally with sufficient accuracy either by weighing or by back scattering
of alpha particles (*cf.*, [76]). Hence we conclude that the unit cell volumes for
silicon and silicon dioxide presented by Kao *et al.* [42] are realistic. We are
now in a position to use this data to calculate eigenstrains.

**2.3** **Modeling the residual strains and stresses**

Obviously, the change in volume during silicon oxidation is considerable and,
consequently, the eigenstrains and eigenstresses will also be very large, at least
in the beginning. It is for this reason, that it is adequate to use strain measures
of *nonlinear* continuum mechanics. Fig. 2.4, which is an adapted form of a
cartoon from Freidin *et al.* [28], illustrates the situation: Originally stress-free
silicon (depicted in cyan) is penetrated by oxygen from the left up to the
dashed line (the reaction front). If the corresponding region were free it would
change its volume (and maybe also its shape) to the stress-free configuration
shown in red on the bottom. We characterize the corresponding deformation
by the deformation gradient **𝐹**^{ch} ≡**𝐹**^{ox} and are inclined to write according to
seemingly standard nonlinear continuum mechanics procedures (see, *e.g.*, [35],
pg. 79 or [60], pg. 73):

*𝜌*0,SiO2 = *𝜌*0,Si

det**𝐹**^{ox}*,* (2.3.1)

where the subscripts 0 refer to the mass densities of silicon dioxide and silicon,
both in a *undeformed* state. However, this formula does*not* apply, because it
holds only if the mass within the material volume is conserved. This, however,
is *not* the case here: Oxygen enters the volume element, causes the chemical
reaction and leads to an increase in mass. Hence, an alternative relation must
hold. In fact, it can take various forms as we shall see now. We start from the
following purely kinematic relation between the unit cell volumes (*cf.*, [60], pg.

64) and find successively:

*𝑉*_{SiO2} =det**𝐹**^{ox}*𝑉*Si ⇒ det**𝐹**^{ox}=

*𝑀*_{SiO2}
*𝑁*_{Avo}

*𝑉*_{SiO2}
*𝑚*_{SiO2}
*𝑀*Si

*𝑁*Avo

*𝑉*Si

*𝑚*Si

≡ *𝑀*_{SiO2}*𝜌*0,Si

*𝑀*Si*𝜌*0,SiO2

≡*𝑣*_{SiO2}
*𝑣*Si

*,* (2.3.2)
because the mass in one silicon or silicon dioxide unit cell is given by *𝑚*Si= *𝑁** ^{𝑀}*Avo

^{Si}

and *𝑚*_{SiO2} =^{𝑀}*𝑁*^{SiO2}_{Avo} , respectively.

Figure 2.4: A schematic of the deformation during silicon oxidation.

On first glance it seems reasonable to assume that amorphous silica is
isotropic and that it expands isotropically when it is created. Hence the
deformation gradient is proportional to the unit tensor,**1**, and we may conclude
that:

**𝐹**^{ox}=*𝐹*^{ox}**1** ⇒ *𝐹*^{ox}= (*𝑣*_{SiO2}
*𝑣*Si

)

1⇑3

*.* (2.3.3)

An appropriate finite strain measure is the Green-Lagrangian strain tensor,
* 𝐸*≡

^{1}2(

**𝐹**^{T}

*−*

**𝐹****1**). From its definition we find

^{2}:

**𝐸**^{ch} ≡**𝐸**^{ox}= ^{1}2⌊︀(*𝑣*_{SiO2}
*𝑣*Si

)

2⇑3

−1}︀**1**≈0*.*36**1.** (2.3.4)
36% is an extremely large strain. However, before we discuss how this extreme
situation is dealt with in the literature, a comment regarding the*isotropy* of the
deformation gradient **𝐹**^{ox} or, more suggestively speaking, on the “volumetric
swelling” during thermal oxidation, is in order. This assumption seems to be
generally accepted in the silicon industry. However, it seems noteworthy that
most recently *anisotropic* swelling during lithiation of Si nanowires has been
observed [48] or be discussed in context with Li-batteries [43]. The reason
for this “is attributed to the interfacial processes of accommodating large
volumetric strains at the lithiation reaction front that depend sensitively on
the crystallographic orientation.” [48] Note that modeling such an effect would

2The letters “ch” are used in [28] to characterize the chemical reaction,*i.e., the oxidation,*
why we use “ox” as a mnemonic.

not necessitate abandoning an isotropic dependence analogously to the one
shown in Eqn. (2.3.4). Rather it will require taking the crystal orientation of
the silicon during the joining procedure into account. The latter is shown in
Fig. 2.4 on the very right indicated by the deformation gradients **𝐹**^{Si} and**𝐹**^{SiO2}.
When modeling silicon oxidation we have to proceed as in the case of lithiation:

The anisotropic elastic material properties of the to-be-oxidized wafer should enter the analysis. However, for simplicity we will ignore this for now and treat the silicon as an isotropic linear elastic material with effective elastic properties.

Clearly, after joining the connected materials will react to the large amount
of strain predicted by Eqn. (2.3.4) and try to accommodate it somehow. There
are various ways. The simplest, from a materials theory point-of-view, is
time-dependent stress relaxation due to visco-elastic behavior. In fact, silicon
dioxide is prone for such behavior if we only think of it as vitreous, *i.e.*, being
in a glassy state. After all, “glasses” are nothing else but silica with certain
additives. We know that they are capable of viscoelastic flow, even at low
temperatures.^{2}

Consequently, viscoelastic models are also used in many publications on
thermal oxidation of silicon. Most surprisingly, 1988 Kao *et al.* used a *genuine*
*fluid mechanics model* of the Newton-Navier-Stokes type in order to capture
the effects of viscosity in their 1988 paper [42]. Their idea was picked up one
year later by Satardja and Oldham [87], who changed their modeling to a
one-dimensional dashpot-spring model for solids of the Maxwell type. A more
detailed, truly multi-axial viscoelastic stress-strain analysis was performed by
Senez *et al.* in 1994 [81]. More recently Lin [46] refers on pg. 8 of his 1999
work [46] to the transformation strain as “viscoplastic,” probably erroneously,
because on pg. 9 he cites the work of Satardja and Oldham and Senez *et al.*,
which is clearly based on viscoelasticity. In any case he characterizes silicon as
non-viscous, linear elastic.

The recent dissertation of Pezyna from 2005 [70] is more precise as far as
terminology is concerned. First of all the importance of SiO2’s susceptibility
to viscous flow is acknowledged (pg. 14): “However, at elevated temperatures,
silica and silicate glasses are not purely elastic solids and can deform in a
viscoelastic manner [*. . .*]” Then an interesting statement follows: “Consequently,
the intrinsic strain is partly accommodated by viscous deformation, allowing
the volume increase to be manifested chiefly as an increase in thickness. The
remaining elastic strain, which will be referred to as the growth strain, *𝜀** _{𝑔}*, gives
rise to the observed growth stress.”

We interpret his words as follows: Initially, the silica expands essentially
freely in perpendicular direction to the constraining silicon. As mentioned
explicitly by Pyzyna[70] on pg. 57 silicon deforms elastically and definitely *not*
viscoelastically or viscoplastically. Note that the main expansion in thickness

2visible, for example, in the thickening at the bottom of old church windows

direction is not an indication for an anisotropy of the eigenstrain, *i.e.*, a non-
spherical form of **𝐹**^{ch} ≡**𝐹**^{ox}. The silicon simply provides an elastic constraint,
so that the main part of deformation due to purely volumetric expansion of
silica goes where there is no constraint, namely perpendicularly to the reaction
front. Clearly, along the interface the stretch will initially be more than allowed
by linear elasticity, simply due to the need of the forming silica for very large
expansion. However, the associated stresses will relax as time goes on and the
stretch will eventually be reduced to the amount allowed by Hooke’s law.

The situation can be understood in terms of the well-known experiments
performed on a viscoelastic strip with Young’s modulus *𝐸*. In the first ex-
periment the strip is suddenly subjected to a dead load, *𝜎*_{0}, which leads to
instantaneous stretching and subsequent relaxation to the amount allotted by
Hooke’s law:

*𝜖*_{ini}= *𝜏*_{𝜎}*𝜏*_{𝜖}

*𝜎*_{0}

*𝐸* → *𝜖*_{H}= *𝜎*_{0}

*𝐸.* (2.3.5)

In a second experiment the beam is suddenly elongated by a fixed amount
in axial direction and then clamped, so that a strain *𝜖*_{0} results. The response is
instantaneous in terms of a tensile stress which will then relax from its initial
value to that dictated by Hooke’s law (*cf.*, [56], pg. 370):

*𝜎*_{ini} = *𝜏*_{𝜖}

*𝜏*_{𝜎}*𝐸𝜖*_{0} → *𝜎*_{H}=*𝐸𝜖*_{0}*.* (2.3.6)
The relaxation is governed by two time parameters, first, the so-called bulk
relaxation time, dealing with relaxation under pure compression, *𝜏** _{𝜖}* =

*𝜂*

*⇑*

_{𝜖}*𝑘*, where

*𝜂*

*𝜖*and

*𝑘*denote the bulk viscosity and the bulk modulus, respectively.

The second time parameter is characteristic for shear loading, *𝜏** _{𝜎}* =

*𝜂*

*⇑*

_{𝜎}*𝐺*,

*𝜂*

*and*

_{𝜎}*𝐺*denoting shear viscosity and shear modulus, respectively. According to Freidin

*et al.*[28] we have

*𝐸*= 60 GPa, Poisson’s ratio

*𝜈*=0

*.*17 , hence

*𝑘*= 3(1−2𝜈)

*≈ 30*

^{𝐸}*.*3 GPa and

*𝐺*= 2(1+𝜈)

*≈ 25*

^{𝐸}*.*6 GPa. Similar numbers and approximately the same trend between them are shown by Dingwell and Webb [18], who report

*𝑘*=43 GPa and

*𝐺*=33 GPa. Surprisingly the trend is reversed in Rao

*et al.*[73], who use

*𝑘*=12

*.*158 GPa and

*𝐺*=40

*.*921 GPa. The correctness of the number for the modulus of compressibility when compared to the shear modulus is hard to believe. Moreover, equations from Dingwell and Webb [18] lead us to conclude that both viscosities are equal. Consequently, due to lack of data, we choose

*𝜂*

*=*

_{𝜎}*𝜂*

*≈2×10*

_{𝜖}^{4}GPa s (at 1000

^{○}C, [81]), which gives

*𝜏**𝜎*⇑^{𝜏}* ^{𝜖}*=

*⇑*

^{𝐺}*≈0*

^{𝑘}*.*84,

*𝜏*

*𝜎*≈780 s, and

*𝜏*

*𝜖*≈660 s. A single relaxation time is presented in [73], namely

*𝜏*

_{SiO}

_{2}=132

*.*49 s. In order to be able to compare it to the times required for the diffusion process, recall the time parameter from the definition of the Fourier number in context with the diffusion (or the heat conduction) equation (

*e.g.*, [12], Chapter 4):

*𝜏*_{diff} = *𝑙*^{2}

*𝐷,* (2.3.7)

where *𝑙* is a characteristic length parameter and *𝐷* the diffusion constant.

Finding a reliable number for the diffusion coefficient of oxygen in silica is
difficult, because the literature is inconclusive. Lin [46], pg. 11 reports *𝐷*=
1*.*83×10^{−14 m}_{s}^{2}, allegedly based on data from the paper of Deal and Grove
[17], who use a constant *𝐵* that is related to*𝐷* but in a complicated manner.

Moreover,*𝐵* is temperature dependent. Thus, it remains unclear how his value
was obtained and under which circumstances it is valid. Rao*et al.*, pg. 374 [73]

use in their simulations a value which is four (!) orders of magnitude larger,
namely *𝐷*=1*.*3786×10^{−10 m}_{s}^{2}. They do not explain where this number comes
from. A typical maximum layer thickness of silica is *𝑙*=2μm (*cf.*, [29]). Hence
we find *𝜏*diff =2*.*9×10^{−2}*. . .*218 s.

In comparison with *𝜏**𝜎* and *𝜏**𝜖* we must conclude that diffusion will either
proceed much faster than the relaxation of stresses and strains due to viscoelastic
effects, or will be of the same order of magnitude. Hence, if we want to
assess *stress-induced diffusion* it is, in principle, necessary to solve the coupled
chemo-mechanical problem in combination with three-dimensional viscoelastic
constitutive equations. This will make the problem explicitly time-dependent
and impossible to solve analytically, even for the simple geometry of a planar
layered structure. On the other hand, we also want to investigate the features of
our stress-assisted diffusion model. They can be explored easily if an analytical
solution for the stresses and strains is available. This, however, is only possible
if we restrict ourselves to linear elasticity, *i.e.*, to Hooke’s law:

* 𝜎*=

*𝜆*Tr(

*−*

**𝜖**

**𝜖**^{ch})

**1**+2

*𝜇*(

*−*

**𝜖**

**𝜖**^{ch})

*,*(2.3.8) where

*is the Cauchy stress tensor and*

**𝜎***refers to the*

**𝜖***linear*strain tensor which is related to the displacement vector

*as follows:*

**𝑢*** 𝜖*=

^{1}

_{2}(∇

*+ ∇*

**𝑢**

**𝑢**^{⊺})

*.*(2.3.9) Obviously the reaction strain

**𝜖**^{ch}must be known numerically before we can proceed with the stress-strain analysis and, what is more, it should be compati- ble with the assumption of small strains,

*i.e.*, it should assume a value in the percent range, at most. As in the case of large deformations,

*cf.*, Eqns. (2.3.3) and (2.3.4), the linear transformation strain is isotropic, hence:

* 𝜎*=

*𝜆*Tr

**𝜖****1**+2

*𝜇*−3

**𝜖***𝑘𝜖*

^{ch}

**1,**(2.3.10) with the bulk modulus being

*𝑘*=

^{1}

_{3}(3

*𝜆*+2

*𝜇*). Freidin

*et al.*[28] choose

*𝜖*

^{ch}=0

*.*03.

Besides a reference to the necessity for small strains and the fact that this
particular value allows them to show an effect of the eigenstesses on diffusion
within their theoretical framework they do not provide any reason for their
choice of this value. However, there is an alternative way for obtaining a number
for*𝜖*^{ch} by using the following relation for small deformations from [60], pg. 232:

*𝜖*^{ch}= *𝜌*0,Si−*𝜌*0,SiO2

3*𝜌*0,SiO2

*.* (2.3.11)

If we insert the data for the mass densities we obtain *𝜖*^{ch} ≈0*.*02. This is
very close to the value from [28]. Note that Eqn. (2.3.11) is a consequence
of Eqn. (2.3.4). To see that we assume, first, that the difference between the
molecular volumes *𝑣*_{SiO2} and *𝑣*Si is small such that we obtain after a Taylor
expansion:

**𝐸**^{ch}≈ *𝑣*_{SiO2}−*𝑣*Si

3*𝑣*Si

**1.** (2.3.12)

Second, we assume that the molar masses are equal, observe Eqn. (2.2.2) and obtain:

**𝐸**^{ch}≈ *𝜌*Si−*𝜌*_{SiO2}

3*𝜌*_{SiO2} **1**≡*𝜖*^{ch}**1.** (2.3.13)
The agreement is not surprising since a relation analogous to Eqn. (2.3.11)
was used in [60] in context with the description of the phase transformation in
Zirconia. Then masses within the unit cells stay constant and the molar mass
does not change. However, in the present case we have *𝑀*Si=28.084_{kmol}^{kg} and
*𝑀*_{SiO2}=60.082_{kmol}^{kg} , which are extremely different. We conclude that it is the
additional mass flow of oxygen into the unit cell that prevents us from using
simple relations as Eqn. (2.3.11) and, in the end, from using linear elasticity
with no hesitation whatsoever.

**2.4** **Intuitive explanations and empirical quantification** **of the impediment encountered during silicon oxi-** **dation**

It was mentioned in Subsection 2.1 that the growth of silicon oxide layers is impeded severely if the insulation windows used in the LOCOS process become very narrow and that the oxide thickness becomes thinner on the edges of the trenches produced in STI. On the other hand, it is well known in mechanics that corners and the closeness of substructures are excellent stress and strain amplifiers. Hence, in view of the huge eigenstrains inherent to silicon oxidation it seems only natural to suspect that the associated stresses and strains in the material might reach a level high enough to influence the course of reaction and diffusion dramatically.

Marcus and Sheng [49] were among the first to emphasize the importance
of stress for silicon oxidation. Shortly after their paper it was directly demon-
strated in 1987 by Huang *et al.* [39] that mechanical stress influences the rate
of silicon oxidation. In two papers in the same and the following year Kao
*et al.* [41] and [42] start modeling the stresses in cylindrical structures and
attempt a coupling between the reaction rate and the radial stress component.

One year later Sutarya and Oldham [87] become even more specific. Following the tradition of materials science they relate the impact of the normal stress,

*𝜎** _{𝑛𝑛}*, and of

*pressure*,

*i.e.*, the trace of stress,

^{Tr}

*𝜎*,

*empirically*to two constitu- tive quantities, first, the surface reaction rate parameter,

*𝑘*

_{s}, and second, the diffusion coefficient,

*𝐷*in terms of an exponential Boltzmann ansatz, namely:

*𝑘*=*𝑘** _{𝑠}*0(

*𝑇*)exp(

*𝜎*

_{𝑛𝑛}*𝑉*

_{𝑘}*𝑘𝑇* ) *, 𝐷*=*𝐷*_{0}(*𝑇*)exp(−*𝑝𝑉*_{𝑑}

*𝑘𝑇* )*,* (2.4.1)
where *𝑘** _{𝑠}*0 and

*𝐷*

_{0}are the temperature dependent reaction and diffusion co- efficients for the stress-free (called “planar” in [87]) case,

*𝑘*is Boltzmann’s constant,

*𝑇*absolute temperature,

*𝑉*

*and*

_{𝑘}*𝑉*

*are two fitting parameters, which have the dimension of a volume. The shear viscosity,*

_{𝑑}*𝜂*, is “adjusted” in a similar manner:

*𝜂*=*𝜂*_{0}(*𝑇*) ^{𝜎}^{𝑠}^{𝑉}^{0}⇑^{2𝑘𝑇}

sinh(^{𝜎}^{𝑠}^{𝑉}^{0}⇑^{2𝑘𝑇})*,* (2.4.2)
where *𝜂*_{0} denotes the shear viscosity the temperature dependent reaction and
diffusion coefficients in the stress-free case, and *𝑉*_{0} is another fitting parameter,
explicitly characterized as such in the paper.

That all of this is a completely heuristic approach, becomes obvious if we try to guess why the authors may have come up with such expressions: On can imagine that a normal stress acting compressively on the reaction front will keep the molecules away from each other and defer the progress of the reaction. It seems also logical to assume that diffusion in a solid under pressure will be procrastinated because the atoms will then be more densely “packed”

and harder to bypass and, finally, viscous Newtonian flow is triggered by shear stress, so the viscosity might depend on it in a nonlinear manner.

Of course, the authors of [87] assume us to be “intelligent” readers with
an intuitive gut feeling to anticipate all that. They scarcely motivate their
approach by saying “The model states that the oxidizing species need to have
enough energy to move the newly formed oxide against the normal force field
*𝜎** _{𝑛𝑛}*. The energy required in a unit reaction is the product of one reaction
jump volume

*𝑉*and

*𝜎*

*𝑛𝑛*. Assuming the Boltzman[n] statistics, the reaction probability varies (with energy) according to the factor exp(

*𝜎*

_{𝑛𝑛}*𝑉*

*⇑*

_{𝑘}*𝑘𝑇*).” It is this concoction of atomistic arguments with field quantities which makes a true continuum scientist used to first principles shudder. However, later we shall use some of these relations and see if and how they alter predictions of a theory in which diffusion and mechanics are coupled but which initially uses stress-independent material coefficients. In other words the mechano-chemical coupling is achieved differently. The next section will explain how.

**2.5** **Driving forces at the reaction front**

From the perspective of modern continuum theory silicon oxidation can be
modeled in terms of a singular interface theory. Such a model is useful if the
interface is relatively sharp, *i.e.*, the fields on the left and right hand side of the

jump in a discontinuous fashion and a high gradient in mass density (say, among other fields) results over a short distance, much smaller than the dimensions of the considered piece of matter. A first attempt in that direction from a mathematical point-of-view was presented in 1994 by Merz and Strecker [50].

They also touch upon an alternative way of modeling silicon oxidation, which could be phase-field theory. However, their primary focus is on mathematical formalities and less on a quantitative physical description.

A major breakthrough in terms of rational continuum theory was presented
recently by Freidin *et al.* [25], [27], [28], [26]. In their papers the idea of
the Eshelby stress tensor, * 𝐵*, being the driving force behind silicon oxidation
was brought to (qualitative) perfection. The specific Eshelby tensor or, more
precisely, the specific Eshelby energy-momentum tensor (in SI-units of J kg

^{−1}), is defined by (

*cf.*, [32], pg. 4 and 25, [47]):

* 𝐵*=

*𝑓*

**1**− 1

*𝜌*_{0}**𝐹**^{⊺}⋅* 𝑃* ⇔

*𝐵*

*𝐴𝐵*=

*𝑓 𝛿*

*𝐴𝐵*− 1

*𝜌*_{0}*𝐹**𝐴**𝑖**𝑃*_{𝑖}*𝐵**,* (2.5.1)
where*𝑓* =*𝑢*−*𝑇 𝑠* denotes the specific free energy density in a material point (*𝑢*
and *𝑠* being the specific internal energy and entropy densities), *𝜌*_{0} is the mass
density of the reference configuration, * 𝐹* denotes the deformation gradient with
its determinant,

*𝐽*=det

*, and*

**𝐹***=*

**𝑃***𝐽*⋅

**𝜎**

**𝐹**^{−⊺}⇔

*𝑃*

_{𝑖}*𝐴*=

*𝐽 𝜎*

*(*

_{𝑖𝑗}*𝐹*

^{−1})

^{⊺}

*𝑗*

*𝐴*≡

*𝐽 𝜎*

_{𝑖𝑗}*𝐹*

_{𝐴}^{−1}

*is the first (nonsymmetric) Piola-Kirchhoff stress tensor, and*

_{𝑗}*denotes the (symmetric) Cauchy stress tensor. Moreover, Eqn. (2.5.1) shows that*

**𝜎***is completely based in the reference configuration (distinguished by a capital symbol and capital Latin indices in contrast to the current configuration which is characterized by small Latin indices for Cartesian coordinates).*

**𝐵**However, silicon oxidation is only one of the more recent applications of
the Eshelby tensor. Originally Eshelby used it for quantifying driving forces on
defects, in particular on (linear) elastic inclusions, see [22], [23]. Shortly after,
or one may say in parallel, the energy-momentum tensor became the playing
ground of the fracture mechanics community, where it arose under the name
J-integral, a term coined by Rice [78], [8]. However, it is fair to say that the
mechanics community simply failed to see the thermodynamic character of the
energy-momentum tensor. This was first acknowledged by Heidug and Lehner
[37]. Other references in the same context are the papers by Truskinovsky [90],
Liu [47], Gurtin [31], Cermelli and Gurtin [13], Müller [55], and and Buratti *et*
*al.* [9].

In these papers it was pointed out that * 𝐵* can be considered as a tensorial
generalization of the scalar chemical potential,

*𝜇*, which is the driving force behind diffusion and reactions in gases and liquids. More precisely, in a reaction where

*𝑖*reactants go in and

*𝑗*products come out, so that in total

*𝑘*=

*𝑖*+

*𝑗*substances are involved, one may define the corresponding

*chemical*

*affinity*in terms of the corresponding chemical potentials,

*𝜇*

*𝑘*, weighted by the

stoichiometric coefficients, *𝑛** _{𝑘}*, and the molar masses,

*𝑀*

*:*

_{𝑘}*𝐴*= − ∑

*𝑘*

*𝑛*_{𝑘}*𝑀*_{𝑘}*𝜇** _{𝑘}*= + ∑

in,𝑖

⋃︀*𝑛** _{𝑖}*⋃︀

*𝑀*

_{𝑖}*𝜇*

*− ∑*

_{𝑖}out,𝑗

*𝑛*_{𝑗}*𝑀*_{𝑗}*𝜇*_{𝑗}*.* (2.5.2)
This notion is explained, for example, in the textbook on chemical thermo-
dynamics by Prigogine and Defay [68], Chapter III, Section 3 ff. and Chapter
IV. If the entropy principle is evaluated for chemical reactions between fluids
and gases one finds that the so-called overall reaction rate, *𝜔*, a “speed,” and
the scalar affinity, *𝐴*, are related by the so-called de Donder inequality and de
Donder equation [67]:

*𝐷*=*𝐴𝜔* ≥0*, 𝜔*=^{→}*𝜔*]︀1−exp(− *𝐴*

*𝑅𝑇*){︀ ≈*𝜔*^{→} *𝐴*

*𝑅𝑇,* (2.5.3)

where *𝐷* is the dissipation and *𝜔*^{→} the forward reaction rate. The latter is
not a vector as the strange chemical engineering notation might lead us to
suspect. The arrow is merely supposed to indicate a forward reaction. In fact,
in equilibrium, for which Eqn. (2.5.3)2 holds, we may write ^{→}*𝜔* =*𝜔*^{←}, the latter
being the backward reaction rate. In the terminology of TIP,^{2} we may simply
say that the de Donder results are nothing else but consequences following from
exploitation of the entropy principle in combination with a linear flux-force
concept. For mechanical engineers it seems worthwhile mentioning that the
forward reaction rate can be interpreted as a volumetric flow of chemicals and,
consequently, carries the units dim^{→}*𝜔*= ^{kmol}_{m}^{3} ^{m}_{s}.

In the aforementioned papers by Freidin *et al.* it was pointed out that,
first, in reactions involving solids the Eshelby tensors assume the role of the
chemical potentials after double scalar multiplication with the normal vector,
* 𝑁*, corresponding to the reference configuration of a surface element of the
reaction front:

*𝜇** _{𝑘}*=

*⋅*

**𝑁**

**𝑀***⋅*

_{𝑘}

**𝑁***,*

**𝑀***∶=*

_{𝑘}

**𝐵**

_{𝑘}*,*(2.5.4) where

**𝑀***is called the*

_{𝑘}*chemical potential tensor*of species

*𝑘*. In fact, in the case of a gas or fluid we may write:

* 𝑀* =

*𝜇1,*(2.5.5)

Second, an analogue to the chemical affinity for solid reactions can be obtained as follows:

*𝐴**𝑁 𝑁* = − ∑

*𝑘*

*𝑛*_{𝑘}*𝑀*_{𝑘}*𝜇** _{𝑘}*≡ − ∑

*𝑘*

*𝑛*_{𝑘}*𝑀*_{𝑘}* 𝑁* ⋅

**𝑀***⋅*

_{𝑘}*(2.5.6) In addition one can also define a chemical affinity tensor by:*

**𝑁**.* 𝐴*= − ∑

*𝑘*

*𝑛*_{𝑘}*𝑀*_{𝑘}**𝑀**_{𝑘}*.* (2.5.7)

2Thermodynamics of Irreversible Processes, see [56].

so that

*𝐴**𝑁 𝑁* =* 𝑁*⋅

*⋅*

**𝐴***(2.5.8)*

**𝑁**.Third, evaluation of the entropy principle allows to show that the dissipation
rate, *𝐷*, is now given by:

*𝐷*=*𝐴**𝑁 𝑁**𝜔**𝑁* ≥0*,* (2.5.9)

where*𝜔**𝑁* is the reaction rate at a surface element of the reaction front with the
reference normal* 𝑁*. The requirement for positive-definiteness of the dissipation
rate is satisfied if we put:

*𝜔**𝑁* =^{→}*𝜔*]︀1−exp(−*𝐴**𝑁 𝑁*

*𝑅𝑇* ){︀ ≈*𝜔*^{→}*𝐴**𝑁 𝑁*

*𝑅𝑇* *,* (2.5.10)

where *𝑅*=8.314_{kmol K}^{kJ} denotes the ideal gas constant and *𝑇* is absolute temper-
ature.

*𝜔**𝑁* is related to the normal propagation speed of the front. To make this
explicit we will now specialize the equations to dry silicon oxidation according
to Eqn. (2.3.2) and obtain from Eqns. (2.5.5) and (2.5.7):

* 𝐴*= ⋃︀

*𝑛*

_{−}⋃︀

*𝑀*

_{−}

**𝑀**_{−}+ ⋃︀

*𝑛*∗⋃︀

*𝑀*∗

*𝜇*∗

**1**−

*𝑛*

_{+}

*𝑀*

_{+}

**𝑀**_{+}≡ (2.5.11)

−J⋃︀*𝑛*⋃︀*𝑀 𝑀*K+ ⋃︀

*𝑛*∗⋃︀

*𝑀*∗

*𝜇*∗

**1,**

where jump brackets, J⋅K, which are frequently used in context with singular interfaces, denote the difference of a quantity on the plus and on the minus side. This implies that all quantities involved are understood as “left” and

“right” limit values and must be evaluated accordingly.

Before we start to detail this equation any further, it is only fair to point out that similar results have been presented in [47], [55], or [56], but not from a chemical engineering point-of-view and not in context with chemical reactions but for mass-conserved phase transformations. If we simplify their results we may write in analogy to Eqns. (2.5.11)2 and Eqns. (2.5.3)1 in terms of a mass flow across the singular interface:

* 𝑁*⋅J

*K⋅*

**𝐵***≥0*

**𝑁**𝜌 𝑊*,*(2.5.12) where

*𝑊*=

*⋅*

**𝑉***is the velocity associated with the flow of mass,*

**𝑁***𝜌𝑉*, normal to the interface, w.r.t. the reference configuration. Hence within the framework of a linear theory we must put as in Eqns. (2.5.10)2:

*𝜌 𝑊* ∼* 𝑁* ⋅J

*K⋅*

**𝐵***(2.5.13)*

**𝑁**.In view of this it is our next goal to rewrite Eqn. (2.5.10)2 in terms of a normal velocity, which will allow us to study the growth and progression of an interface explicitly. However, in order to do that we must first introduce some kinematic relations pertinent to our reaction.

**2.6** **Mathematical treatment of silicon oxidation – The** **full picture**

**2.6.1** **Relevant kinematic quantities**

We will now go through the statements on kinematics made by Freidin *et al.*

[25], [27], [28], [26] for a simple reason. For the sake of brevity the details in that paper had to be kept to a minimum and many things were left unsaid to be read between the lines. We also warn our readers to be ready to accept a notation which looks clumsy on first glance but which has proven to be necessary when studying chemical reactions of the kind specified in Eqn. (2.1.1).

Figure 2.5: Kinematics of the solid-gas-solid reaction *𝑛*−*𝐵*−+*𝑛*∗*𝐵*∗⇌*𝑛*+*𝐵*+.
Recall the general reaction shown in Eqn. (2.1.1) and consider the corre-
sponding situation depicted in Fig. 2.5. In the configuration on the very right
the gas “∗” has penetrated the solid skeleton region *𝜐*+2 up to the current
interface, which is identifiable by a thick black line, *𝛾*. The region beyond
that line, *𝜐*−, still contains original not reacted material. Due to the volume
expansion both regions will deform and carry stresses and strains.

In order to characterize the deformation we consider two current linear
segments, d* 𝑥*+∈

*𝜐*+ and d

*−∈*

**𝑥***𝜐*−, in both regions. We wish to link them to line segments in unstressed solid reference configurations.

*Two*such configurations come to mind. The first one consists of a solid completely made of “−” material.

It is shown on the upper left of the figure. The second one is a solid consisting
exclusively of the product material, “+.” It is shown on the lower left. Note
that in both reference configurations we have indicated the images, *𝛤* and
*𝛤*^{∗}, of the current interface, *𝛾*, by black dotted lines. Clearly these are purely
geometrical, unphysical objects. However, they allow us to identify four image
volumes of *𝜐*±. These are denoted by *𝑉*± and *𝑉*_{±}^{∗}, respectively. Again, they are
purely geometrical objects. They are related to reference configurations, hence,
the capital letters. Moreover, the upper index “∗” is used to distinguish both
sets from each other *and* to indicate that the second set is made of the reaction
product due to the chemical reaction between the “−” material and the gaseous

2Note that we denote quantities of the current configuration by small letters.

agent “∗.” We are now in a position to link four linear line segments in the two
reference configurations, d* 𝑋*± and d

**𝑋**^{∗}

_{±}, by means of deformation gradients,

*, as follows:*

**𝐹**d**𝑥**_{±} =* 𝐹*±⋅d

*±*

**𝑋***,*d

*±=*

**𝑥**

**𝐹**^{∗}

_{±}⋅d

**𝑋**^{∗}

_{±}(2.6.1) with d

*±∈*

**𝑥***𝜐*±, d

*±∈*

**𝑋***𝑉*±, and d

**𝑋**^{∗}

_{±}∈

*𝑉*

_{±}

^{∗}. All of the mappings (

*i.e.*, deformation gradients) used in these equations are shown in Fig. 2.5. From Eqns. (2.6.1) we get in the usual fashion Nanson formulae for the directed surface elements:

d*𝑎*_{±}**𝑛**_{±}=*𝐽*_{±}d*𝐴*_{±}**𝐹**^{−⊺}_{±} ⋅**𝑁**_{±}*,* d*𝑎*_{±}**𝑛**_{±}=*𝐽*_{±}^{∗}d*𝐴*^{∗}_{±} **𝐹**^{∗−⊺}_{±} ⋅**𝑁**^{∗}_{±} (2.6.2)
and transformation relations for the volume elements:

d*𝜐*_{±} =*𝐽*_{±}d*𝑉*_{±}*,* d*𝜐*_{±}=*𝐽*_{±}^{∗}d*𝑉*_{±}^{∗}*,* (2.6.3)
where*𝐽* denote the determinants of the deformation gradients,*e.g.*,*𝐽*_{−}^{∗}=det**𝐹**^{∗}_{−}.

There is yet another mapping shown in the figure, namely* 𝐹*∗. Note that it
was not entitled

**𝐹**^{∗}

_{±}, because it relates the stress-free reference configuration of the chemically unaffected to the fully affected one, independently of the regions

*𝑉*± and

*𝑉*

_{±}

^{∗}. The symbol “∗” was used to emphasize the relevance of the gaseous agent during the reaction.

Consequently, between the volume elements of the two stress free reference configurations the following relations hold:

d*𝑉*_{±}^{∗}=*𝐽*∗d*𝑉*_{±}*, 𝐽*∗=det* 𝐹*∗

*.*(2.6.4) Moreover, as usual, multiplicative decomposition applies:

**𝐹**_{±} =**𝐹**^{∗}_{±}⋅* 𝐹*∗ ⇒

*𝐽*

_{±}=

*𝐽*

_{±}

^{∗}

*𝐽*∗

*.*(2.6.5) Note that Eqns. (2.6.4) and (2.6.5) are consistent with Eqns. (2.6.3) for we may write:

d*𝜐*_{±}=*𝐽*_{±}d*𝑉*_{±} =*𝐽*_{±}^{∗}*𝐽*∗d*𝑉*_{±} ≡*𝐽*_{±}^{∗}d*𝑉*_{±}^{∗}*.* (2.6.6)
**2.6.2** **Mass densities**

We now turn to the definition and calculation of several mass densities in the
various configurations. This will be based on the conservation or addition
of mass to the various volume elements involved. We start by saying that
we consider the mass densities of the two stress free reference configurations,
*𝑉* =*𝑉*+∪*𝑉*− and *𝑉*^{∗} =*𝑉*_{+}^{∗}∪*𝑉*_{−}^{∗}, as given and we denote them by *𝜌*_{0−} and*𝜌*^{∗}_{0+}^{2},

2Note that in this case we depart from our convention that capital letters signal quantities
in the reference configuration. The capital Greek letter rho looks like a*𝑃*, which makes it
difficult to recognize as a mass density. To make both ends meet we have decided to use an
index 0 for indicating the reference configuration.